# Electronic Supplementary Material (ESI) for Dalton Transactions.
# This journal is © The Royal Society of Chemistry 2023

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_a
_database_code_depnum_ccdc_archive 'CCDC 2213277'
loop_
_audit_author_name
_audit_author_address
'Maxim Molokeev'
;Kirensky Institute of Physics Federal Research Center KSC SB RAS
Russia
;
_audit_update_record             
;
2022-10-17 deposited with the CCDC.	2023-01-13 downloaded from the CCDC.
;

_diffrn_radiation_probe          x-ray
_diffrn_measurement_device_type  
;
D8 ADVANCE Bruker
;
_pd_spec_mount_mode              reflection
_pd_meas_scan_method             step
loop_
_diffrn_radiation_wavelength
_diffrn_radiation_wavelength_wt
1.5406 1.0000
1.5443 0.5000
_diffrn_radiation_type           
;
 Cu K\a~1~~2~
;
_diffrn_radiation_monochromator  none

_chemical_name_mineral           
;
;

_symmetry_space_group_name_H-M   P12/c1

_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_hall  
;
-P 2yc
;

_cell_length_a                   7.52262(10)
_cell_length_b                   5.26905(8)
_cell_length_c                   11.22463(16)
_cell_angle_alpha                90
_cell_angle_beta                 104.6413(7)
_cell_angle_gamma                90
_cell_volume                     430.463(11)
_chemical_formula_moiety         
;
Lu2 O6 W
;
_chemical_formula_sum            
;
Lu2 O6 W
;

_chemical_formula_weight         629.78
_cell_formula_units_Z            4
_exptl_crystal_density_diffrn    9.7175(2)

_exptl_absorpt_coefficient_mu    132.995

_cell_measurement_temperature    300
_diffrn_ambient_temperature      300


_pd_char_colour                  
;
colourless
;

_cell_measurement_reflns_used    104
_cell_measurement_theta_min      2.5
_cell_measurement_theta_max      45
_pd_proc_number_of_points        4250
_pd_meas_2theta_range_min        5
_pd_meas_2theta_range_max        90
_pd_meas_2theta_range_inc        0.02

_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_pref_orient_corr     
;
Anisotropic model of PO. Spherical harmonics 2 ordrer.
 Jarvinen (1993). Application of symmetrized harmonics expansion to correction
of the preferred orientation effect. - J. Appl. Cryst. 26 p525-531.
;

_refine_ls_shift/su_max          0.01000
_refine_ls_R_I_factor            1.1
_pd_proc_ls_prof_wR_factor       5.61
_pd_proc_ls_prof_R_factor        4.04
_pd_proc_ls_prof_wR_expected     1.38
_refine_ls_goodness_of_fit_all   4.05
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z '
'-x, y, -z+1/2 '
'x, -y, z+1/2 '
'-x, -y, -z '
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_B_iso_or_equiv
Lu1 Lu 0 0.7372(5) 0.25 1 0.63(14)
Lu2 Lu 0.5 0.6840(5) 0.25 1 0.55(14)
Lu3 Lu 0.2016(2) 0.1874(4) 0.07864(15) 1 0.58(14)
W1 W 0.2802(2) 0.2549(4) 0.38720(14) 1 0.80(14)
O1 O 0.356(3) 0.135(4) 0.5525(19) 1 1.1(2)
O2 O 0.507(3) 0.374(3) 0.3862(17) 1 1.1(2)
O3 O 0.151(3) 0.525(4) 0.442(2) 1 1.1(2)
O4 O 0.276(3) -0.014(3) 0.2665(18) 1 1.1(2)
O5 O 0.070(3) 0.034(4) 0.3981(17) 1 1.1(2)
O6 O 0.197(3) 0.467(3) 0.2220(18) 1 1.1(2)

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Lu1 O3 2.438(21) .
Lu1 O4 2.422(17) 1_565
Lu1 O5 2.245(19) 1_565
Lu1 O6 2.134(16) .
Lu2 O1 2.404(20) 3_564
Lu2 O2 2.228(17) .
Lu2 O4 2.358(16) 1_565
Lu2 O6 2.497(17) .
Lu3 O1 2.119(19) 3_554
Lu3 O2 2.343(17) 2_655
Lu3 O3 3.153(18) 2_555
Lu3 O3 2.120(21) 3_564
Lu3 O4 2.299(18) .
Lu3 O5 2.272(18) 2_555
Lu3 O5 2.330(19) 3_554
Lu3 O6 2.188(17) .
W1 O1 1.905(20) .
W1 O1 3.351(18) 4_656
W1 O2 1.820(17) .
W1 O2 3.285(17) 4_666
W1 O3 1.910(19) .
W1 O4 1.955(17) .
W1 O5 1.991(19) .
W1 O6 2.119(18) .


loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O1 W1 O1 64.66(53) . 4_656
O1 W1 O2 94.01(40) . .
O1 W1 O2 58.42(63) . 4_666
O1 W1 O3 89.13(44) . .
O1 W1 O4 112.51(56) . .
O1 W1 O5 78.07(43) . .
O2 Lu2 O1 148.2(14) . 3_564
O2 Lu2 O1 74.41(41) . 4_666
O2 Lu2 O2 85.74(32) . 2_655
O2 Lu2 O4 109.51(41) . 1_565
O2 Lu2 O4 130.90(72) . 2_665
O2 Lu2 O6 67.25(44) . .
O2 Lu2 O6 73.47(38) . 2_655
O2 W1 O1 94.01(40) . .
O2 W1 O1 59.59(56) . 4_656
O2 W1 O2 61.68(53) . 4_666
O2 W1 O3 107.39(46) . .
O2 W1 O4 95.54(38) . .
O2 W1 O6 83.27(38) . .
O3 Lu1 O3 125.42(75) . 2_555
O3 Lu1 O4 88.95(31) . 1_565
O3 Lu1 O4 120.95(59) . 2_565
O3 Lu1 O5 72.26(45) . 1_565
O3 Lu1 O6 68.82(47) . .
O3 Lu1 O6 75.50(40) . 2_555
O3 W1 O1 89.13(44) . .
O3 W1 O1 147.9(14) . 4_656
O3 W1 O2 107.39(46) . .
O3 W1 O2 59.70(60) . 4_666
O3 W1 O4 147.4(14) . .
O3 W1 O5 86.51(40) . .
O3 W1 O6 80.04(43) . .
O4 Lu3 O1 75.06(42) . 3_554
O4 Lu3 O2 92.21(31) . 2_655
O4 Lu3 O3 109.44(41) . 2_555
O4 Lu3 O5 75.40(39) . 2_555
O4 Lu3 O5 121.17(61) . 3_554
O4 Lu3 O6 71.44(43) . .
O4 W1 O1 112.51(56) . .
O4 W1 O1 64.21(50) . 4_656
O4 W1 O2 95.54(38) . .
O4 W1 O2 152.5(15) . 4_666
O4 W1 O3 147.4(14) . .
O4 W1 O5 75.23(44) . .
O4 W1 O6 80.00(39) . .
O5 W1 O1 78.07(43) . .
O5 W1 O1 104.46(38) . 4_656
O5 W1 O2 122.62(61) . 4_666
O5 W1 O3 86.51(40) . .
O5 W1 O4 75.23(44) . .
O5 W1 O6 107.36(45) . .
O6 Lu1 O3 68.82(47) . .
O6 Lu1 O3 75.50(40) . 2_555
O6 Lu1 O4 76.03(36) . 1_565
O6 Lu1 O5 122.12(62) . 1_565
O6 Lu1 O5 113.39(49) . 2_565
O6 Lu1 O6 96.34(33) . 2_555
O6 Lu2 O1 83.19(32) . 3_564
O6 Lu2 O1 118.78(55) . 4_666
O6 Lu2 O2 67.25(44) . .
O6 Lu2 O2 73.47(38) . 2_655
O6 Lu2 O4 70.81(38) . 1_565
O6 Lu2 O6 125.51(60) . 2_655
O6 Lu3 O1 138.7(10) . 3_554
O6 Lu3 O2 77.38(36) . 2_655
O6 Lu3 O3 60.32(54) . 2_555
O6 Lu3 O3 90.99(37) . 3_564
O6 Lu3 O4 71.44(43) . .
O6 Lu3 O5 88.46(34) . 2_555
O6 Lu3 O5 153.3(17) . 3_554
O6 W1 O1 123.05(60) . 4_656
O6 W1 O2 83.27(38) . .
O6 W1 O2 109.98(41) . 4_666
O6 W1 O3 80.04(43) . .
O6 W1 O4 80.00(39) . .
O6 W1 O5 107.36(45) . .
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_a_CCDC1
_database_code_depnum_ccdc_archive 'CCDC 2213278'
loop_
_audit_author_name
_audit_author_address
'Maxim Molokeev'
;Kirensky Institute of Physics Federal Research Center KSC SB RAS
Russia
;
_audit_update_record             
;
2022-10-17 deposited with the CCDC.	2023-01-13 downloaded from the CCDC.
;

_diffrn_radiation_probe          x-ray
_diffrn_measurement_device_type  
;
D8 ADVANCE Bruker
;
_pd_spec_mount_mode              reflection
_pd_meas_scan_method             step
loop_
_diffrn_radiation_wavelength
_diffrn_radiation_wavelength_wt
1.5406 1.0000
1.5443 0.5000
_diffrn_radiation_type           
;
 Cu K\a~1~~2~
;
_diffrn_radiation_monochromator  none

_chemical_name_mineral           
;
;

_symmetry_space_group_name_H-M   C12/c1

_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_hall  
;
-C 2yc
;

_cell_length_a                   16.39881(15)
_cell_length_b                   11.17398(10)
_cell_length_c                   5.43037(5)
_cell_angle_alpha                90
_cell_angle_beta                 107.6698(5)
_cell_angle_gamma                90
_cell_volume                     948.116(15)
_chemical_formula_moiety         
;
Gd15.68 Lu0.32 O48 W8
;
_chemical_formula_sum            
;
Gd15.68 Lu0.32 O48 W8
;

_chemical_formula_weight         4760.39
_cell_formula_units_Z            1
_exptl_crystal_density_diffrn    8.337

_exptl_absorpt_coefficient_mu    219.993

_cell_measurement_temperature    300
_diffrn_ambient_temperature      300


_pd_char_colour                  
;
colourless
;

_cell_measurement_reflns_used    104
_cell_measurement_theta_min      2.5
_cell_measurement_theta_max      45
_pd_proc_number_of_points        4250
_pd_meas_2theta_range_min        5
_pd_meas_2theta_range_max        90
_pd_meas_2theta_range_inc        0.02

_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_pref_orient_corr     
;
Anisotropic model of PO. Spherical harmonics 2 ordrer.
 Jarvinen (1993). Application of symmetrized harmonics expansion to correction
of the preferred orientation effect. - J. Appl. Cryst. 26 p525-531.
;

_refine_ls_shift/su_max          0.01000
_refine_ls_R_I_factor            0.81
_pd_proc_ls_prof_wR_factor       3.12
_pd_proc_ls_prof_R_factor        2.25
_pd_proc_ls_prof_wR_expected     1.24
_refine_ls_goodness_of_fit_all   2.52
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z '
'-x, y, -z+1/2 '
'x, -y, z+1/2 '
'-x, -y, -z '
'x+1/2, y+1/2, z '
'-x+1/2, y+1/2, -z+1/2 '
'x+1/2, -y+1/2, z+1/2 '
'-x+1/2, -y+1/2, -z '
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_B_iso_or_equiv
Lu1 Lu 0.5 0.1084(5) 0.75 0.07(7) 1.7(3)
Gd1 Gd 0.5 0.1084(5) 0.75 0.93(7) 1.7(3)
Lu2 Lu 0 0.1328(4) 0.75 0.01(5) 1.4(3)
Gd2 Gd 0 0.1328(4) 0.75 0.99(5) 1.4(3)
Gd3 Gd 0.3275(3) 0.1150(4) 0.1135(9) 1.00(5) 1.49(19)
W1 W 0.1535(2) 0.1467(3) 0.4367(8) 1 1.66(17)
O1 O 0.236(2) 0.046(3) 0.402(8) 1 2.6(3)
O2 O 0.087(2) 0.039(3) 0.472(7) 1 2.6(3)
O3 O 0.234(2) 0.216(3) 0.730(7) 1 2.6(3)
O4 O 0.113(2) 0.212(3) 0.167(8) 1 2.6(3)
O5 O 0.084(3) 0.264(2) 0.598(10) 1 2.6(3)
O6 O 0.598(2) 0.013(2) 0.604(10) 1 2.6(3)

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Lu1 O4 2.858(28) 7_555
Lu1 O5 2.433(42) 7_555
Lu1 O6 2.262(24) .
Lu1 O6 2.498(40) 3_555
Gd1 O4 2.858(28) 7_555
Gd1 O5 2.433(42) 7_555
Gd1 O6 2.262(24) .
Gd1 O6 2.498(40) 3_555
Lu2 O2 2.592(28) .
Lu2 O2 2.475(32) 3_555
Lu2 O4 2.607(37) 1_556
Lu2 O5 2.327(32) .
Gd2 O2 2.592(28) .
Gd2 O2 2.475(32) 3_555
Gd2 O4 2.607(37) 1_556
Gd2 O5 2.327(32) .
Gd3 O1 2.593(30) .
Gd3 O1 2.400(33) 3_554
Gd3 O3 2.454(34) 1_554
Gd3 O3 2.413(31) 8_556
Gd3 O4 2.812(33) 8_555
Gd3 O5 2.237(39) 8_556
Gd3 O6 2.250(30) 2_655
Gd3 O6 2.180(38) 4_656
W1 O1 1.812(26) .
W1 O1 3.282(37) 3_555
W1 O2 1.673(28) .
W1 O2 3.192(35) 3_554
W1 O3 1.898(33) .
W1 O3 2.755(27) 8_556
W1 O4 1.589(39) .
W1 O5 2.095(33) .


loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O1 Gd3 O1 70.97(70) . 3_554
O1 Gd3 O3 108.80(72) . 1_554
O1 Gd3 O3 68.88(71) . 8_556
O1 Gd3 O4 152.9(27) . 8_555
O1 Gd3 O5 97.34(67) . 8_556
O1 Gd3 O6 132.2(13) . 2_655
O1 Gd3 O6 71.53(78) . 4_656
O1 W1 O1 61.7(10) . 3_555
O1 W1 O2 95.64(65) . .
O1 W1 O2 66.48(90) . 3_554
O1 W1 O3 89.40(71) . .
O1 W1 O3 73.51(63) . 8_556
O1 W1 O4 107.77(93) . .
O2 Lu2 O2 132.3(12) . 2_556
O2 Lu2 O2 68.43(72) . 3_555
O2 Lu2 O2 74.96(61) . 4_556
O2 Lu2 O4 105.74(64) . 1_556
O2 Lu2 O4 90.18(50) . 2_555
O2 Lu2 O5 63.80(88) . .
O2 Gd2 O2 132.3(12) . 2_556
O2 Gd2 O2 68.43(72) . 3_555
O2 Gd2 O2 74.96(61) . 4_556
O2 Gd2 O4 105.74(64) . 1_556
O2 Gd2 O4 90.18(50) . 2_555
O2 Gd2 O5 63.80(88) . .
O2 W1 O1 95.64(65) . .
O2 W1 O1 64.58(96) . 3_555
O2 W1 O2 62.93(99) . 3_554
O2 W1 O3 120.5(11) . .
O2 W1 O4 109.32(97) . .
O2 W1 O5 86.89(64) . .
O3 W1 O1 89.40(71) . .
O3 W1 O1 66.58(92) . 3_555
O3 W1 O2 120.5(11) . .
O3 W1 O3 71.57(70) . 8_556
O3 W1 O4 125.1(15) . .
O3 W1 O5 73.86(88) . .
O4 W1 O1 107.77(93) . .
O4 W1 O2 109.32(97) . .
O4 W1 O2 67.8(10) . 3_554
O4 W1 O3 125.1(15) . .
O4 W1 O3 64.90(94) . 8_556
O4 W1 O5 88.27(84) . .
O5 Lu2 O2 63.80(88) . .
O5 Lu2 O2 110.20(74) . 3_555
O5 Lu2 O2 129.1(13) . 4_556
O5 Lu2 O4 75.70(76) . 1_556
O5 Lu2 O4 79.59(71) . 2_555
O5 Lu2 O5 101.92(64) . 2_556
O5 Gd2 O2 63.80(88) . .
O5 Gd2 O2 110.20(74) . 3_555
O5 Gd2 O2 129.1(13) . 4_556
O5 Gd2 O4 75.70(76) . 1_556
O5 Gd2 O4 79.59(71) . 2_555
O5 Gd2 O5 101.92(64) . 2_556
O5 W1 O1 103.76(73) . 3_555
O5 W1 O2 86.89(64) . .
O5 W1 O2 129.6(14) . 3_554
O5 W1 O3 73.86(88) . .
O5 W1 O3 107.00(68) . 8_556
O5 W1 O4 88.27(84) . .
O6 Lu1 O4 73.27(51) . 7_555
O6 Lu1 O5 104.67(76) . 7_555
O6 Lu1 O5 107.38(81) . 8_556
O6 Lu1 O6 123.79(85) . 2_656
O6 Lu1 O6 69.78(80) . 3_555
O6 Lu1 O6 80.44(64) . 4_656
O6 Gd1 O4 73.27(51) . 7_555
O6 Gd1 O5 104.67(76) . 7_555
O6 Gd1 O5 107.38(81) . 8_556
O6 Gd1 O6 123.79(85) . 2_656
O6 Gd1 O6 69.78(80) . 3_555
O6 Gd1 O6 80.44(64) . 4_656
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_a_CCDC2
_database_code_depnum_ccdc_archive 'CCDC 2213280'
loop_
_audit_author_name
_audit_author_address
'Maxim Molokeev'
;Kirensky Institute of Physics Federal Research Center KSC SB RAS
Russia
;
_audit_update_record             
;
2022-10-17 deposited with the CCDC.	2023-01-13 downloaded from the CCDC.
;

_diffrn_radiation_probe          x-ray
_diffrn_measurement_device_type  
;
D8 ADVANCE Bruker
;
_pd_spec_mount_mode              reflection
_pd_meas_scan_method             step
loop_
_diffrn_radiation_wavelength
_diffrn_radiation_wavelength_wt
1.5406 1.0000
1.5443 0.5000
_diffrn_radiation_type           
;
 Cu K\a~1~~2~
;
_diffrn_radiation_monochromator  none

_chemical_name_mineral           
;
;

_symmetry_space_group_name_H-M   C12/c1

_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_hall  
;
-C 2yc
;

_cell_length_a                   16.3383(4)
_cell_length_b                   11.1340(3)
_cell_length_c                   5.39850(14)
_cell_angle_alpha                90
_cell_angle_beta                 107.7554(11)
_cell_angle_gamma                90
_cell_volume                     935.26(4)
_chemical_formula_moiety         
;
Gd13.40 Lu2.60 O48 W8
;
_chemical_formula_sum            
;
Gd13.40 Lu2.60 O48 W8
;

_chemical_formula_weight         4800.79
_cell_formula_units_Z            1
_exptl_crystal_density_diffrn    8.524

_exptl_absorpt_coefficient_mu    208.388

_cell_measurement_temperature    300
_diffrn_ambient_temperature      300


_pd_char_colour                  
;
colourless
;

_cell_measurement_reflns_used    104
_cell_measurement_theta_min      2.5
_cell_measurement_theta_max      35
_pd_proc_number_of_points        3250
_pd_meas_2theta_range_min        5
_pd_meas_2theta_range_max        70
_pd_meas_2theta_range_inc        0.02

_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_pref_orient_corr     
;
Anisotropic model of PO. Spherical harmonics 2 ordrer.
 Jarvinen (1993). Application of symmetrized harmonics expansion to correction
of the preferred orientation effect. - J. Appl. Cryst. 26 p525-531.
;

_refine_ls_shift/su_max          0.01000
_refine_ls_R_I_factor            0.66
_pd_proc_ls_prof_wR_factor       4.04
_pd_proc_ls_prof_R_factor        3.21
_pd_proc_ls_prof_wR_expected     2.7
_refine_ls_goodness_of_fit_all   1.5
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z '
'-x, y, -z+1/2 '
'x, -y, z+1/2 '
'-x, -y, -z '
'x+1/2, y+1/2, z '
'-x+1/2, y+1/2, -z+1/2 '
'x+1/2, -y+1/2, z+1/2 '
'-x+1/2, -y+1/2, -z '
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_B_iso_or_equiv
Lu1 Lu 0.5 0.1066(8) 0.75 0.25(10) 2.0(6)
Gd1 Gd 0.5 0.1066(8) 0.75 0.75(10) 2.0(6)
Gd2 Gd 0 0.1329(7) 0.75 1.00(9) 2.0(6)
Lu3 Lu 0.3285(4) 0.1136(5) 0.1144(13) 0.20(9) 1.9(4)
Gd3 Gd 0.3285(4) 0.1136(5) 0.1144(13) 0.80(9) 1.9(4)
W1 W 0.1543(3) 0.1451(4) 0.4346(11) 1 1.9(3)
O1 O 0.246(3) 0.045(5) 0.388(10) 1 0.6(5)
O2 O 0.066(3) 0.039(3) 0.463(10) 1 0.6(5)
O3 O 0.227(3) 0.201(4) 0.738(9) 1 0.6(5)
O4 O 0.100(3) 0.218(4) 0.120(13) 1 0.6(5)
O5 O 0.094(4) 0.259(3) 0.598(13) 1 0.6(5)
O6 O 0.604(3) 0.012(3) 0.570(9) 1 0.6(5)

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Lu1 O4 2.770(40) 7_555
Lu1 O5 2.523(54) 7_555
Lu1 O6 2.438(36) .
Lu1 O6 2.413(40) 3_555
Gd1 O4 2.770(40) 7_555
Gd1 O5 2.523(54) 7_555
Gd1 O6 2.438(36) .
Gd1 O6 2.413(40) 3_555
Gd2 O2 2.382(41) .
Gd2 O2 2.322(38) 3_555
Gd2 O4 2.359(58) 1_556
Gd2 O5 2.402(44) .
Lu3 O1 2.407(42) .
Lu3 O1 2.328(51) 3_554
Lu3 O3 2.402(44) 1_554
Lu3 O3 2.481(43) 8_556
Lu3 O4 2.717(45) 8_555
Lu3 O5 2.197(52) 8_556
Lu3 O6 2.038(37) 2_655
Lu3 O6 2.220(41) 4_656
Gd3 O1 2.407(42) .
Gd3 O1 2.328(51) 3_554
Gd3 O3 2.402(44) 1_554
Gd3 O3 2.481(43) 8_556
Gd3 O4 2.717(45) 8_555
Gd3 O5 2.197(52) 8_556
Gd3 O6 2.038(37) 2_655
Gd3 O6 2.220(41) 4_656
W1 O1 1.944(42) .
W1 O1 3.237(52) 3_555
W1 O2 1.906(33) .
W1 O2 3.244(44) 3_554
W1 O3 1.815(44) .
W1 O3 2.944(39) 8_556
W1 O4 1.846(62) .
W1 O5 1.971(45) .


loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O1 Lu3 O1 74.85(99) . 3_554
O1 Lu3 O3 106.03(94) . 1_554
O1 Lu3 O3 74.87(93) . 8_556
O1 Lu3 O5 94.65(94) . 8_556
O1 Lu3 O6 127.6(16) . 2_655
O1 Lu3 O6 64.4(12) . 4_656
O1 Gd3 O1 74.85(99) . 3_554
O1 Gd3 O3 106.03(94) . 1_554
O1 Gd3 O3 74.87(93) . 8_556
O1 Gd3 O5 94.65(94) . 8_556
O1 Gd3 O6 127.6(16) . 2_655
O1 Gd3 O6 64.4(12) . 4_656
O1 W1 O1 61.6(14) . 3_555
O1 W1 O2 106.68(96) . .
O1 W1 O2 73.2(10) . 3_554
O1 W1 O3 89.72(95) . .
O1 W1 O3 71.62(96) . 8_556
O1 W1 O4 107.8(12) . .
O2 Gd2 O2 127.9(16) . 2_556
O2 Gd2 O2 74.12(85) . 3_555
O2 Gd2 O2 63.2(11) . 4_556
O2 Gd2 O4 113.1(12) . 1_556
O2 Gd2 O4 87.68(82) . 2_555
O2 Gd2 O5 64.5(12) . .
O2 W1 O1 106.68(96) . .
O2 W1 O1 73.80(95) . 3_555
O2 W1 O2 60.3(12) . 3_554
O2 W1 O3 116.2(13) . .
O2 W1 O4 100.55(100) . .
O2 W1 O5 82.46(85) . .
O3 W1 O1 89.72(95) . .
O3 W1 O1 61.1(15) . 3_555
O3 W1 O2 116.2(13) . .
O3 W1 O3 76.88(87) . 8_556
O3 W1 O4 132.6(26) . .
O3 W1 O5 69.7(14) . .
O4 W1 O1 107.8(12) . .
O4 W1 O2 100.55(100) . .
O4 W1 O2 65.2(15) . 3_554
O4 W1 O3 132.6(26) . .
O4 W1 O3 68.3(12) . 8_556
O4 W1 O5 87.8(11) . .
O5 Gd2 O2 64.5(12) . .
O5 Gd2 O2 113.7(10) . 3_555
O5 Gd2 O2 124.1(14) . 4_556
O5 Gd2 O4 72.8(11) . 1_556
O5 Gd2 O4 79.97(94) . 2_555
O5 Gd2 O5 108.47(99) . 2_556
O5 W1 O1 105.1(11) . 3_555
O5 W1 O2 82.46(85) . .
O5 W1 O2 126.4(17) . 3_554
O5 W1 O3 69.7(14) . .
O5 W1 O3 103.56(88) . 8_556
O5 W1 O4 87.8(11) . .
O6 Lu1 O4 70.55(82) . 7_555
O6 Lu1 O5 102.29(83) . 7_555
O6 Lu1 O5 107.41(95) . 8_556
O6 Lu1 O6 128.8(14) . 2_656
O6 Lu1 O6 67.97(94) . 3_555
O6 Lu1 O6 84.40(67) . 4_656
O6 Gd1 O4 70.55(82) . 7_555
O6 Gd1 O5 102.29(83) . 7_555
O6 Gd1 O5 107.41(95) . 8_556
O6 Gd1 O6 128.8(14) . 2_656
O6 Gd1 O6 67.97(94) . 3_555
O6 Gd1 O6 84.40(67) . 4_656
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_a_CCDC3
_database_code_depnum_ccdc_archive 'CCDC 2213279'
loop_
_audit_author_name
_audit_author_address
'Maxim Molokeev'
;Kirensky Institute of Physics Federal Research Center KSC SB RAS
Russia
;
_audit_update_record             
;
2022-10-17 deposited with the CCDC.	2023-01-13 downloaded from the CCDC.
;

_diffrn_radiation_probe          x-ray
_diffrn_measurement_device_type  
;
D8 ADVANCE Bruker
;
_pd_spec_mount_mode              reflection
_pd_meas_scan_method             step
loop_
_diffrn_radiation_wavelength
_diffrn_radiation_wavelength_wt
1.5406 1.0000
1.5443 0.5000
_diffrn_radiation_type           
;
 Cu K\a~1~~2~
;
_diffrn_radiation_monochromator  none

_chemical_name_mineral           
;
;

_symmetry_space_group_name_H-M   P12/c1

_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_hall  
;
-P 2yc
;

_cell_length_a                   7.56643(11)
_cell_length_b                   5.30847(9)
_cell_length_c                   11.30437(17)
_cell_angle_alpha                90
_cell_angle_beta                 104.5274(9)
_cell_angle_gamma                90
_cell_volume                     439.536(12)
_chemical_formula_moiety         
;
Gd1.96 Lu6.04 O24 W4
;
_chemical_formula_sum            
;
Gd1.96 Lu6.04 O24 W4
;

_chemical_formula_weight         2484.39
_cell_formula_units_Z            1
_exptl_crystal_density_diffrn    9.4633(3)

_exptl_absorpt_coefficient_mu    157.006

_cell_measurement_temperature    300
_diffrn_ambient_temperature      300


_pd_char_colour                  
;
colourless
;

_cell_measurement_reflns_used    104
_cell_measurement_theta_min      2.5
_cell_measurement_theta_max      35
_pd_proc_number_of_points        3250
_pd_meas_2theta_range_min        5
_pd_meas_2theta_range_max        70
_pd_meas_2theta_range_inc        0.02

_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_pref_orient_corr     
;
Anisotropic model of PO. Spherical harmonics 2 ordrer.
 Jarvinen (1993). Application of symmetrized harmonics expansion to correction
of the preferred orientation effect. - J. Appl. Cryst. 26 p525-531.
;

_refine_ls_shift/su_max          0.01000
_refine_ls_R_I_factor            0.0
_pd_proc_ls_prof_wR_factor       4.78
_pd_proc_ls_prof_R_factor        3.76
_pd_proc_ls_prof_wR_expected     2.91
_refine_ls_goodness_of_fit_all   1.64
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z '
'-x, y, -z+1/2 '
'x, -y, z+1/2 '
'-x, -y, -z '
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_B_iso_or_equiv
Lu1 Lu 0 0.7353(9) 0.25 0.92(9) 1.7(3)
Gd1 Gd 0 0.7353(9) 0.25 0.08(9) 1.7(3)
Lu2 Lu 0.5 0.6836(9) 0.25 0.50(7) 1.3(3)
Gd2 Gd 0.5 0.6836(9) 0.25 0.50(7) 1.3(3)
Lu3 Lu 0.2001(3) 0.1910(6) 0.0779(2) 0.80(8) 1.5(3)
Gd3 Gd 0.2001(3) 0.1910(6) 0.0779(2) 0.20(8) 1.5(3)
W1 W 0.2790(3) 0.2538(6) 0.3873(2) 1 1.6(3)
O1 O 0.342(4) 0.133(6) 0.548(3) 1 1.9(4)
O2 O 0.506(4) 0.368(5) 0.382(2) 1 1.9(4)
O3 O 0.150(4) 0.532(6) 0.435(3) 1 1.9(4)
O4 O 0.273(5) -0.016(4) 0.272(3) 1 1.9(4)
O5 O 0.069(4) 0.046(6) 0.399(3) 1 1.9(4)
O6 O 0.211(5) 0.457(4) 0.222(3) 1 1.9(4)

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Lu1 O3 2.373(32) .
Lu1 O4 2.411(27) 1_565
Lu1 O5 2.321(32) 1_565
Lu1 O6 2.255(26) .
Gd1 O3 2.373(32) .
Gd1 O4 2.411(27) 1_565
Gd1 O5 2.321(32) 1_565
Gd1 O6 2.255(26) .
Lu2 O1 2.494(32) 3_564
Lu2 O2 2.236(24) .
Lu2 O4 2.401(26) 1_565
Lu2 O6 2.445(27) .
Gd2 O1 2.494(32) 3_564
Gd2 O2 2.236(24) .
Gd2 O4 2.401(26) 1_565
Gd2 O6 2.445(27) .
Lu3 O1 2.099(29) 3_554
Lu3 O2 2.351(24) 2_655
Lu3 O3 3.181(25) 2_555
Lu3 O3 2.146(32) 3_564
Lu3 O4 2.391(30) .
Lu3 O5 2.252(23) 2_555
Lu3 O5 2.377(32) 3_554
Lu3 O6 2.141(28) .
Gd3 O1 2.099(29) 3_554
Gd3 O2 2.351(24) 2_655
Gd3 O3 3.181(25) 2_555
Gd3 O3 2.146(32) 3_564
Gd3 O4 2.391(30) .
Gd3 O5 2.252(23) 2_555
Gd3 O5 2.377(32) 3_554
Gd3 O6 2.141(28) .
W1 O1 1.871(32) .
W1 O1 3.452(26) 4_656
W1 O2 1.836(24) .
W1 O2 3.368(24) 4_666
W1 O3 1.920(29) .
W1 O4 1.929(27) .
W1 O5 1.965(25) .
W1 O6 2.106(30) .


loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O1 W1 O1 66.10(75) . 4_656
O1 W1 O2 97.59(53) . .
O1 W1 O2 59.79(91) . 4_666
O1 W1 O3 90.83(66) . .
O1 W1 O4 111.00(87) . .
O1 W1 O5 75.86(70) . .
O2 Lu2 O1 145.9(19) . 3_564
O2 Lu2 O1 75.92(57) . 4_666
O2 Lu2 O2 82.96(48) . 2_655
O2 Lu2 O4 108.88(60) . 1_565
O2 Lu2 O4 132.1(11) . 2_665
O2 Lu2 O6 65.52(70) . .
O2 Lu2 O6 71.17(60) . 2_655
O2 Gd2 O1 145.9(19) . 3_564
O2 Gd2 O1 75.92(57) . 4_666
O2 Gd2 O2 82.96(48) . 2_655
O2 Gd2 O4 108.88(60) . 1_565
O2 Gd2 O4 132.1(11) . 2_665
O2 Gd2 O6 65.52(70) . .
O2 Gd2 O6 71.17(60) . 2_655
O2 W1 O1 97.59(53) . .
O2 W1 O1 57.95(83) . 4_656
O2 W1 O2 63.55(69) . 4_666
O2 W1 O3 107.49(65) . .
O2 W1 O4 94.97(58) . .
O2 W1 O6 79.88(58) . .
O3 Lu1 O3 125.9(12) . 2_555
O3 Lu1 O4 87.14(48) . 1_565
O3 Lu1 O4 123.20(97) . 2_565
O3 Lu1 O5 73.32(70) . 1_565
O3 Lu1 O6 68.09(73) . .
O3 Lu1 O6 77.13(59) . 2_555
O3 Gd1 O3 125.9(12) . 2_555
O3 Gd1 O4 87.14(48) . 1_565
O3 Gd1 O4 123.20(97) . 2_565
O3 Gd1 O5 73.32(70) . 1_565
O3 Gd1 O6 68.09(73) . .
O3 Gd1 O6 77.13(59) . 2_555
O3 W1 O1 90.83(66) . .
O3 W1 O1 148.3(20) . 4_656
O3 W1 O2 107.49(65) . .
O3 W1 O2 60.33(86) . 4_666
O3 W1 O4 146.4(20) . .
O3 W1 O5 86.34(57) . .
O3 W1 O6 80.04(64) . .
O4 Lu3 O1 76.21(63) . 3_554
O4 Lu3 O2 90.99(44) . 2_655
O4 Lu3 O3 107.53(58) . 2_555
O4 Lu3 O5 75.15(63) . 2_555
O4 Lu3 O5 119.23(94) . 3_554
O4 Lu3 O6 69.45(73) . .
O4 Gd3 O1 76.21(63) . 3_554
O4 Gd3 O2 90.99(44) . 2_655
O4 Gd3 O3 107.53(58) . 2_555
O4 Gd3 O5 75.15(63) . 2_555
O4 Gd3 O5 119.23(94) . 3_554
O4 Gd3 O6 69.45(73) . .
O4 W1 O1 111.00(87) . .
O4 W1 O1 65.11(73) . 4_656
O4 W1 O2 94.97(58) . .
O4 W1 O2 152.9(23) . 4_666
O4 W1 O3 146.4(20) . .
O4 W1 O5 75.31(70) . .
O4 W1 O6 79.73(63) . .
O5 W1 O1 75.86(70) . .
O5 W1 O1 107.12(56) . 4_656
O5 W1 O2 121.58(86) . 4_666
O5 W1 O3 86.34(57) . .
O5 W1 O4 75.31(70) . .
O5 W1 O6 108.98(75) . .
O6 Lu1 O3 68.09(73) . .
O6 Lu1 O3 77.13(59) . 2_555
O6 Lu1 O4 75.80(55) . 1_565
O6 Lu1 O5 121.94(94) . 1_565
O6 Lu1 O5 113.69(74) . 2_565
O6 Lu1 O6 98.13(51) . 2_555
O6 Gd1 O3 68.09(73) . .
O6 Gd1 O3 77.13(59) . 2_555
O6 Gd1 O4 75.80(55) . 1_565
O6 Gd1 O5 121.94(94) . 1_565
O6 Gd1 O5 113.69(74) . 2_565
O6 Gd1 O6 98.13(51) . 2_555
O6 Lu2 O1 82.29(49) . 3_564
O6 Lu2 O1 121.20(91) . 4_666
O6 Lu2 O2 65.52(70) . .
O6 Lu2 O2 71.17(60) . 2_655
O6 Lu2 O4 72.57(58) . 1_565
O6 Lu2 O6 121.07(87) . 2_655
O6 Gd2 O1 82.29(49) . 3_564
O6 Gd2 O1 121.20(91) . 4_666
O6 Gd2 O2 65.52(70) . .
O6 Gd2 O2 71.17(60) . 2_655
O6 Gd2 O4 72.57(58) . 1_565
O6 Gd2 O6 121.07(87) . 2_655
O6 Lu3 O1 137.6(15) . 3_554
O6 Lu3 O2 74.67(58) . 2_655
O6 Lu3 O3 62.12(78) . 2_555
O6 Lu3 O3 94.96(58) . 3_564
O6 Lu3 O4 69.45(73) . .
O6 Lu3 O5 90.03(56) . 2_555
O6 Gd3 O1 137.6(15) . 3_554
O6 Gd3 O2 74.67(58) . 2_655
O6 Gd3 O3 62.12(78) . 2_555
O6 Gd3 O3 94.96(58) . 3_564
O6 Gd3 O4 69.45(73) . .
O6 Gd3 O5 90.03(56) . 2_555
O6 W1 O1 119.83(84) . 4_656
O6 W1 O2 79.88(58) . .
O6 W1 O2 110.15(62) . 4_666
O6 W1 O3 80.04(64) . .
O6 W1 O4 79.73(63) . .
O6 W1 O5 108.98(75) . .
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_a_CCDC4
_database_code_depnum_ccdc_archive 'CCDC 2213281'
loop_
_audit_author_name
_audit_author_address
'Maxim Molokeev'
;Kirensky Institute of Physics Federal Research Center KSC SB RAS
Russia
;
_audit_update_record             
;
2022-10-17 deposited with the CCDC.	2023-01-13 downloaded from the CCDC.
;

_diffrn_radiation_probe          x-ray
_diffrn_measurement_device_type  
;
D8 ADVANCE Bruker
;
_pd_spec_mount_mode              reflection
_pd_meas_scan_method             step
loop_
_diffrn_radiation_wavelength
_diffrn_radiation_wavelength_wt
1.5406 1.0000
1.5443 0.5000
_diffrn_radiation_type           
;
 Cu K\a~1~~2~
;
_diffrn_radiation_monochromator  none

_chemical_name_mineral           
;
;

_symmetry_space_group_name_H-M   P12/c1

_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_hall  
;
-P 2yc
;

_cell_length_a                   7.52747(14)
_cell_length_b                   5.27346(11)
_cell_length_c                   11.2307(2)
_cell_angle_alpha                90
_cell_angle_beta                 104.6381(11)
_cell_angle_gamma                90
_cell_volume                     431.341(14)
_chemical_formula_moiety         
;
Gd0.60 Lu7.40 O24 W4
;
_chemical_formula_sum            
;
Gd0.60 Lu7.40 O24 W4
;

_chemical_formula_weight         2508.49
_cell_formula_units_Z            1
_exptl_crystal_density_diffrn    9.6978(3)

_exptl_absorpt_coefficient_mu    141.071

_cell_measurement_temperature    300
_diffrn_ambient_temperature      300


_pd_char_colour                  
;
colourless
;

_cell_measurement_reflns_used    104
_cell_measurement_theta_min      2.5
_cell_measurement_theta_max      35
_pd_proc_number_of_points        3250
_pd_meas_2theta_range_min        5
_pd_meas_2theta_range_max        70
_pd_meas_2theta_range_inc        0.02

_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_pref_orient_corr     
;
Anisotropic model of PO. Spherical harmonics 2 ordrer.
 Jarvinen (1993). Application of symmetrized harmonics expansion to correction
of the preferred orientation effect. - J. Appl. Cryst. 26 p525-531.
;

_refine_ls_shift/su_max          0.01000
_refine_ls_R_I_factor            2.28
_pd_proc_ls_prof_wR_factor       6.8
_pd_proc_ls_prof_R_factor        5.19
_pd_proc_ls_prof_wR_expected     2.83
_refine_ls_goodness_of_fit_all   2.4
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z '
'-x, y, -z+1/2 '
'x, -y, z+1/2 '
'-x, -y, -z '
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_B_iso_or_equiv
Lu1 Lu 0 0.7304(9) 0.25 0.77(8) 3.2(3)
Gd1 Gd 0 0.7304(9) 0.25 0.23(8) 3.2(3)
Lu2 Lu 0.5 0.6840(9) 0.25 0.93(9) 3.4(3)
Gd2 Gd 0.5 0.6840(9) 0.25 0.07(9) 3.4(3)
Lu3 Lu 0.2031(3) 0.1892(8) 0.0775(2) 1.00(10) 4.2(3)
W1 W 0.2819(3) 0.2577(7) 0.3876(2) 1 3.8(3)
O1 O 0.300(4) 0.108(7) 0.559(3) 1 4.3(4)
O2 O 0.509(4) 0.372(5) 0.386(2) 1 4.3(4)
O3 O 0.141(4) 0.582(6) 0.426(3) 1 4.3(4)
O4 O 0.268(5) -0.015(4) 0.262(2) 1 4.3(4)
O5 O 0.102(5) 0.051(6) 0.398(3) 1 4.3(4)
O6 O 0.257(5) 0.422(5) 0.231(3) 1 4.3(4)

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Lu1 O3 2.141(31) .
Lu1 O4 2.398(29) 1_565
Lu1 O5 2.359(32) 1_565
Lu1 O6 2.577(28) .
Gd1 O3 2.141(31) .
Gd1 O4 2.398(29) 1_565
Gd1 O5 2.359(32) 1_565
Gd1 O6 2.577(28) .
Lu2 O1 2.537(32) 3_564
Lu2 O2 2.234(24) .
Lu2 O4 2.388(27) 1_565
Lu2 O6 2.259(28) .
Gd2 O1 2.537(32) 3_564
Gd2 O2 2.234(24) .
Gd2 O4 2.388(27) 1_565
Gd2 O6 2.259(28) .
Lu3 O1 1.762(34) 3_554
Lu3 O2 2.311(24) 2_655
Lu3 O3 3.309(26) 2_555
Lu3 O3 2.041(32) 3_564
Lu3 O4 2.275(21) .
Lu3 O5 2.490(29) 2_555
Lu3 O5 2.339(32) 3_554
Lu3 O6 2.071(30) .
W1 O1 2.052(33) .
W1 O2 1.817(24) .
W1 O2 3.276(23) 4_666
W1 O3 2.113(29) .
W1 O4 1.998(21) .
W1 O5 1.765(30) .
W1 O6 1.926(31) .


loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O1 W1 O2 107.28(63) . .
O1 W1 O2 66.20(76) . 4_666
O1 W1 O3 92.15(64) . .
O1 W1 O4 111.36(77) . .
O1 W1 O5 64.57(95) . .
O2 Lu2 O1 143.6(18) . 3_564
O2 Lu2 O1 80.29(54) . 4_666
O2 Lu2 O2 85.15(46) . 2_655
O2 Lu2 O4 110.30(59) . 1_565
O2 Lu2 O4 129.1(10) . 2_665
O2 Lu2 O6 59.87(85) . .
O2 Lu2 O6 66.49(72) . 2_655
O2 Gd2 O1 143.6(18) . 3_564
O2 Gd2 O1 80.29(54) . 4_666
O2 Gd2 O2 85.15(46) . 2_655
O2 Gd2 O4 110.30(59) . 1_565
O2 Gd2 O4 129.1(10) . 2_665
O2 Gd2 O6 59.87(85) . .
O2 Gd2 O6 66.49(72) . 2_655
O2 W1 O1 107.28(63) . .
O2 W1 O2 62.69(71) . 4_666
O2 W1 O3 104.80(61) . .
O2 W1 O4 96.50(60) . .
O2 W1 O6 73.53(68) . .
O3 Lu1 O3 137.1(17) . 2_555
O3 Lu1 O4 86.50(44) . 1_565
O3 Lu1 O4 118.03(82) . 2_565
O3 Lu1 O5 67.32(83) . 1_565
O3 Lu1 O6 68.80(71) . .
O3 Lu1 O6 84.27(52) . 2_555
O3 Gd1 O3 137.1(17) . 2_555
O3 Gd1 O4 86.50(44) . 1_565
O3 Gd1 O4 118.03(82) . 2_565
O3 Gd1 O5 67.32(83) . 1_565
O3 Gd1 O6 68.80(71) . .
O3 Gd1 O6 84.27(52) . 2_555
O3 W1 O1 92.15(64) . .
O3 W1 O2 104.80(61) . .
O3 W1 O2 61.75(80) . 4_666
O3 W1 O4 141.8(16) . .
O3 W1 O5 93.05(62) . .
O3 W1 O6 83.35(62) . .
O4 Lu3 O1 71.74(77) . 3_554
O4 Lu3 O2 93.43(48) . 2_655
O4 Lu3 O3 107.11(56) . 2_555
O4 Lu3 O5 75.68(62) . 2_555
O4 Lu3 O5 118.46(82) . 3_554
O4 Lu3 O6 64.58(76) . .
O4 W1 O1 111.36(77) . .
O4 W1 O2 96.50(60) . .
O4 W1 O3 141.8(16) . .
O4 W1 O5 72.43(77) . .
O4 W1 O6 72.76(66) . .
O5 W1 O1 64.57(95) . .
O5 W1 O2 122.88(98) . 4_666
O5 W1 O3 93.05(62) . .
O5 W1 O4 72.43(77) . .
O5 W1 O6 116.02(97) . .
O6 Lu1 O3 68.80(71) . .
O6 Lu1 O3 84.27(52) . 2_555
O6 Lu1 O4 73.71(59) . 1_565
O6 Lu1 O5 113.14(75) . 1_565
O6 Lu1 O5 120.75(93) . 2_565
O6 Lu1 O6 101.74(51) . 2_555
O6 Gd1 O3 68.80(71) . .
O6 Gd1 O3 84.27(52) . 2_555
O6 Gd1 O4 73.71(59) . 1_565
O6 Gd1 O5 113.14(75) . 1_565
O6 Gd1 O5 120.75(93) . 2_565
O6 Gd1 O6 101.74(51) . 2_555
O6 Lu2 O1 83.75(53) . 3_564
O6 Lu2 O1 129.6(12) . 4_666
O6 Lu2 O2 59.87(85) . .
O6 Lu2 O2 66.49(72) . 2_655
O6 Lu2 O4 79.96(54) . 1_565
O6 Lu2 O6 104.58(61) . 2_655
O6 Gd2 O1 83.75(53) . 3_564
O6 Gd2 O1 129.6(12) . 4_666
O6 Gd2 O2 59.87(85) . .
O6 Gd2 O2 66.49(72) . 2_655
O6 Gd2 O4 79.96(54) . 1_565
O6 Gd2 O6 104.58(61) . 2_655
O6 Lu3 O1 128.6(14) . 3_554
O6 Lu3 O2 68.13(70) . 2_655
O6 Lu3 O3 68.09(70) . 2_555
O6 Lu3 O3 107.38(77) . 3_564
O6 Lu3 O4 64.58(76) . .
O6 Lu3 O5 94.22(56) . 2_555
O6 W1 O2 73.53(68) . .
O6 W1 O2 110.92(68) . 4_666
O6 W1 O3 83.35(62) . .
O6 W1 O4 72.76(66) . .
O6 W1 O5 116.02(97) . .
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_a_CCDC5
_database_code_depnum_ccdc_archive 'CCDC 2213282'
loop_
_audit_author_name
_audit_author_address
'Maxim Molokeev'
;Kirensky Institute of Physics Federal Research Center KSC SB RAS
Russia
;
_audit_update_record             
;
2022-10-17 deposited with the CCDC.	2023-01-13 downloaded from the CCDC.
;

_diffrn_radiation_probe          x-ray
_diffrn_measurement_device_type  
;
D8 ADVANCE Bruker
;
_pd_spec_mount_mode              reflection
_pd_meas_scan_method             step
loop_
_diffrn_radiation_wavelength
_diffrn_radiation_wavelength_wt
1.5406 1.0000
1.5443 0.5000
_diffrn_radiation_type           
;
 Cu K\a~1~~2~
;
_diffrn_radiation_monochromator  none

_chemical_name_mineral           
;
;

_symmetry_space_group_name_H-M   P12/c1

_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_hall  
;
-P 2yc
;

_cell_length_a                   7.54138(16)
_cell_length_b                   5.28624(12)
_cell_length_c                   11.2588(3)
_cell_angle_alpha                90
_cell_angle_beta                 104.5927(13)
_cell_angle_gamma                90
_cell_volume                     434.359(17)
_chemical_formula_moiety         
;
Gd0.80 Lu7.20 O24 W4
;
_chemical_formula_sum            
;
Gd0.80 Lu7.20 O24 W4
;

_chemical_formula_weight         2504.94
_cell_formula_units_Z            1
_exptl_crystal_density_diffrn    9.576

_exptl_absorpt_coefficient_mu    142.853

_cell_measurement_temperature    300
_diffrn_ambient_temperature      300


_pd_char_colour                  
;
colourless
;

_cell_measurement_reflns_used    104
_cell_measurement_theta_min      2.5
_cell_measurement_theta_max      35
_pd_proc_number_of_points        3250
_pd_meas_2theta_range_min        5
_pd_meas_2theta_range_max        70
_pd_meas_2theta_range_inc        0.02

_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_pref_orient_corr     
;
Anisotropic model of PO. Spherical harmonics 2 ordrer.
 Jarvinen (1993). Application of symmetrized harmonics expansion to correction
of the preferred orientation effect. - J. Appl. Cryst. 26 p525-531.
;

_refine_ls_shift/su_max          0.01000
_refine_ls_R_I_factor            0.0
_pd_proc_ls_prof_wR_factor       6.57
_pd_proc_ls_prof_R_factor        4.61
_pd_proc_ls_prof_wR_expected     3.02
_refine_ls_goodness_of_fit_all   2.18
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z '
'-x, y, -z+1/2 '
'x, -y, z+1/2 '
'-x, -y, -z '
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_B_iso_or_equiv
Lu1 Lu 0 0.7361(11) 0.25 0.92(11) 1.2(4)
Gd1 Gd 0 0.7361(11) 0.25 0.08(11) 1.2(4)
Lu2 Lu 0.5 0.6852(10) 0.25 0.68(9) 0.6(4)
Gd2 Gd 0.5 0.6852(10) 0.25 0.32(9) 0.6(4)
Lu3 Lu 0.2016(4) 0.1895(8) 0.0777(3) 1.00(11) 1.8(4)
W1 W 0.2797(4) 0.2547(7) 0.3867(3) 1 1.4(4)
O1 O 0.325(5) 0.106(8) 0.529(4) 1 1.7(5)
O2 O 0.516(5) 0.376(6) 0.392(3) 1 1.7(5)
O3 O 0.125(5) 0.541(8) 0.434(4) 1 1.7(5)
O4 O 0.273(7) -0.030(5) 0.268(3) 1 1.7(5)
O5 O 0.059(5) 0.031(6) 0.382(3) 1 1.7(5)
O6 O 0.216(6) 0.465(5) 0.221(3) 1 1.7(5)

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Lu1 O3 2.293(42) .
Lu1 O4 2.366(40) 1_565
Lu1 O5 2.122(32) 1_565
Lu1 O6 2.254(33) .
Gd1 O3 2.293(42) .
Gd1 O4 2.366(40) 1_565
Gd1 O5 2.122(32) 1_565
Gd1 O6 2.254(33) .
Lu2 O1 2.737(42) 3_564
Lu2 O2 2.268(32) .
Lu2 O4 2.326(37) 1_565
Lu2 O6 2.386(34) .
Gd2 O1 2.737(42) 3_564
Gd2 O2 2.268(32) .
Gd2 O4 2.326(37) 1_565
Gd2 O6 2.386(34) .
Lu3 O1 1.965(38) 3_554
Lu3 O2 2.292(29) 2_655
Lu3 O3 3.061(33) 2_555
Lu3 O3 2.123(43) 3_564
Lu3 O4 2.376(31) .
Lu3 O5 2.284(29) 2_555
Lu3 O5 2.485(32) 3_554
Lu3 O6 2.155(30) .
W1 O1 1.739(43) .
W1 O1 3.463(33) 4_656
W1 O2 1.880(29) .
W1 O2 3.233(32) 4_666
W1 O3 2.061(37) .
W1 O4 2.004(29) .
W1 O5 2.031(30) .
W1 O6 2.120(31) .


loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O1 W1 O1 62.8(11) . 4_656
O1 W1 O2 99.21(74) . .
O1 W1 O2 67.5(10) . 4_666
O1 W1 O3 94.95(87) . .
O1 W1 O4 103.93(94) . .
O1 W1 O5 74.36(85) . .
O2 Lu2 O1 149.1(28) . 3_564
O2 Lu2 O1 73.86(77) . 4_666
O2 Lu2 O2 87.79(58) . 2_655
O2 Lu2 O4 108.33(73) . 1_565
O2 Lu2 O4 128.1(13) . 2_665
O2 Lu2 O6 68.37(78) . .
O2 Lu2 O6 70.46(74) . 2_655
O2 Gd2 O1 149.1(28) . 3_564
O2 Gd2 O1 73.86(77) . 4_666
O2 Gd2 O2 87.79(58) . 2_655
O2 Gd2 O4 108.33(73) . 1_565
O2 Gd2 O4 128.1(13) . 2_665
O2 Gd2 O6 68.37(78) . .
O2 Gd2 O6 70.46(74) . 2_655
O2 W1 O1 99.21(74) . .
O2 W1 O1 55.6(11) . 4_656
O2 W1 O2 60.39(96) . 4_666
O2 W1 O3 109.56(81) . .
O2 W1 O4 98.14(81) . .
O2 W1 O6 81.48(73) . .
O3 Lu1 O3 126.5(16) . 2_555
O3 Lu1 O4 90.39(55) . 1_565
O3 Lu1 O4 117.5(11) . 2_565
O3 Lu1 O5 74.44(84) . 1_565
O3 Lu1 O6 72.38(79) . .
O3 Lu1 O6 74.38(75) . 2_555
O3 Gd1 O3 126.5(16) . 2_555
O3 Gd1 O4 90.39(55) . 1_565
O3 Gd1 O4 117.5(11) . 2_565
O3 Gd1 O5 74.44(84) . 1_565
O3 Gd1 O6 72.38(79) . .
O3 Gd1 O6 74.38(75) . 2_555
O3 W1 O1 94.95(87) . .
O3 W1 O1 146.8(24) . 4_656
O3 W1 O2 109.56(81) . .
O3 W1 O2 63.1(10) . 4_666
O3 W1 O4 143.3(22) . .
O3 W1 O5 85.45(64) . .
O3 W1 O6 79.91(79) . .
O4 Lu3 O1 81.24(79) . 3_554
O4 Lu3 O2 94.86(66) . 2_655
O4 Lu3 O3 109.40(80) . 2_555
O4 Lu3 O5 69.67(83) . 2_555
O4 Lu3 O5 121.3(10) . 3_554
O4 Lu3 O6 72.41(71) . .
O4 W1 O1 103.93(94) . .
O4 W1 O1 69.19(86) . 4_656
O4 W1 O2 98.14(81) . .
O4 W1 O2 153.3(28) . 4_666
O4 W1 O3 143.3(22) . .
O4 W1 O5 70.29(88) . .
O4 W1 O6 81.08(64) . .
O5 W1 O1 74.36(85) . .
O5 W1 O1 109.24(70) . 4_656
O5 W1 O2 126.8(12) . 4_666
O5 W1 O3 85.45(64) . .
O5 W1 O4 70.29(88) . .
O5 W1 O6 106.24(76) . .
O6 Lu1 O3 72.38(79) . .
O6 Lu1 O3 74.38(75) . 2_555
O6 Lu1 O4 72.52(81) . 1_565
O6 Lu1 O5 122.4(11) . 1_565
O6 Lu1 O5 113.40(83) . 2_565
O6 Lu1 O6 101.05(66) . 2_555
O6 Gd1 O3 72.38(79) . .
O6 Gd1 O3 74.38(75) . 2_555
O6 Gd1 O4 72.52(81) . 1_565
O6 Gd1 O5 122.4(11) . 1_565
O6 Gd1 O5 113.40(83) . 2_565
O6 Gd1 O6 101.05(66) . 2_555
O6 Lu2 O1 82.05(55) . 3_564
O6 Lu2 O1 122.1(12) . 4_666
O6 Lu2 O2 68.37(78) . .
O6 Lu2 O2 70.46(74) . 2_655
O6 Lu2 O4 70.90(84) . 1_565
O6 Lu2 O6 121.6(11) . 2_655
O6 Gd2 O1 82.05(55) . 3_564
O6 Gd2 O1 122.1(12) . 4_666
O6 Gd2 O2 68.37(78) . .
O6 Gd2 O2 70.46(74) . 2_655
O6 Gd2 O4 70.90(84) . 1_565
O6 Gd2 O6 121.6(11) . 2_655
O6 Lu3 O1 143.8(23) . 3_554
O6 Lu3 O2 74.24(73) . 2_655
O6 Lu3 O3 60.69(100) . 2_555
O6 Lu3 O3 93.99(72) . 3_564
O6 Lu3 O4 72.41(71) . .
O6 Lu3 O5 89.01(62) . 2_555
O6 W1 O1 121.2(10) . 4_656
O6 W1 O2 81.48(73) . .
O6 W1 O2 108.64(69) . 4_666
O6 W1 O3 79.91(79) . .
O6 W1 O4 81.08(64) . .
O6 W1 O5 106.24(76) . .
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_a_CCDC6
_database_code_depnum_ccdc_archive 'CCDC 2213283'
loop_
_audit_author_name
_audit_author_address
'Maxim Molokeev'
;Kirensky Institute of Physics Federal Research Center KSC SB RAS
Russia
;
_audit_update_record             
;
2022-10-17 deposited with the CCDC.	2023-01-13 downloaded from the CCDC.
;

_diffrn_radiation_probe          x-ray
_diffrn_measurement_device_type  
;
D8 ADVANCE Bruker
;
_pd_spec_mount_mode              reflection
_pd_meas_scan_method             step
loop_
_diffrn_radiation_wavelength
_diffrn_radiation_wavelength_wt
1.5406 1.0000
1.5443 0.5000
_diffrn_radiation_type           
;
 Cu K\a~1~~2~
;
_diffrn_radiation_monochromator  none

_chemical_name_mineral           
;
;

_symmetry_space_group_name_H-M   P12/c1

_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_hall  
;
-P 2yc
;

_cell_length_a                   7.53287(10)
_cell_length_b                   5.27787(8)
_cell_length_c                   11.24076(15)
_cell_angle_alpha                90
_cell_angle_beta                 104.6241(8)
_cell_angle_gamma                90
_cell_volume                     432.426(10)
_chemical_formula_moiety         
;
Gd0.36 Lu7.64 O24 W4
;
_chemical_formula_sum            
;
Gd0.36 Lu7.64 O24 W4
;

_chemical_formula_weight         2512.74
_cell_formula_units_Z            1
_exptl_crystal_density_diffrn    9.6326(2)

_exptl_absorpt_coefficient_mu    137.387

_cell_measurement_temperature    300
_diffrn_ambient_temperature      300


_pd_char_colour                  
;
colourless
;

_cell_measurement_reflns_used    104
_cell_measurement_theta_min      2.5
_cell_measurement_theta_max      45
_pd_proc_number_of_points        4250
_pd_meas_2theta_range_min        5
_pd_meas_2theta_range_max        90
_pd_meas_2theta_range_inc        0.02

_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_pref_orient_corr     
;
Anisotropic model of PO. Spherical harmonics 2 ordrer.
 Jarvinen (1993). Application of symmetrized harmonics expansion to correction
of the preferred orientation effect. - J. Appl. Cryst. 26 p525-531.
;

_refine_ls_shift/su_max          0.01000
_refine_ls_R_I_factor            1.09
_pd_proc_ls_prof_wR_factor       5.92
_pd_proc_ls_prof_R_factor        4.51
_pd_proc_ls_prof_wR_expected     1.42
_refine_ls_goodness_of_fit_all   4.17
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z '
'-x, y, -z+1/2 '
'x, -y, z+1/2 '
'-x, -y, -z '
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_B_iso_or_equiv
Lu1 Lu 0 0.7375(6) 0.25 0.98(7) 0.77(17)
Gd1 Gd 0 0.7375(6) 0.25 0.02(7) 0.77(17)
Lu2 Lu 0.5 0.6844(6) 0.25 1.00(5) 1.1(2)
Lu3 Lu 0.2009(3) 0.1876(4) 0.07863(17) 0.92(6) 0.63(16)
Gd3 Gd 0.2009(3) 0.1876(4) 0.07863(17) 0.08(6) 0.63(16)
W1 W 0.2796(2) 0.2548(4) 0.38722(16) 1 1.00(16)
O1 O 0.353(3) 0.130(4) 0.548(2) 1 1.6(3)
O2 O 0.508(3) 0.370(4) 0.382(2) 1 1.6(3)
O3 O 0.155(4) 0.521(5) 0.446(3) 1 1.6(3)
O4 O 0.269(4) -0.009(4) 0.264(2) 1 1.6(3)
O5 O 0.075(3) 0.038(5) 0.403(2) 1 1.6(3)
O6 O 0.199(4) 0.462(4) 0.226(2) 1 1.6(3)

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Lu1 O3 2.494(30) .
Lu1 O4 2.399(23) 1_565
Lu1 O5 2.302(24) 1_565
Lu1 O6 2.153(23) .
Gd1 O3 2.494(30) .
Gd1 O4 2.399(23) 1_565
Gd1 O5 2.302(24) 1_565
Gd1 O6 2.153(23) .
Lu2 O1 2.464(21) 3_564
Lu2 O2 2.216(21) .
Lu2 O4 2.410(23) 1_565
Lu2 O6 2.506(23) .
Lu3 O1 2.107(19) 3_554
Lu3 O2 2.332(17) 2_655
Lu3 O3 3.160(23) 2_555
Lu3 O3 2.108(29) 3_564
Lu3 O4 2.267(21) .
Lu3 O5 2.280(18) 2_555
Lu3 O5 2.295(23) 3_554
Lu3 O6 2.203(21) .
Gd3 O1 2.107(19) 3_554
Gd3 O2 2.332(17) 2_655
Gd3 O3 3.160(23) 2_555
Gd3 O3 2.108(29) 3_564
Gd3 O4 2.267(21) .
Gd3 O5 2.280(18) 2_555
Gd3 O5 2.295(23) 3_554
Gd3 O6 2.203(21) .
W1 O1 1.871(21) .
W1 O1 3.361(18) 4_656
W1 O2 1.839(17) .
W1 O2 3.333(21) 4_666
W1 O3 1.898(25) .
W1 O4 1.951(21) .
W1 O5 1.963(20) .
W1 O6 2.071(21) .


loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O1 W1 O1 63.36(56) . 4_656
O1 W1 O2 95.53(44) . .
O1 W1 O2 59.39(68) . 4_666
O1 W1 O3 88.61(57) . .
O1 W1 O4 112.55(61) . .
O1 W1 O5 75.80(50) . .
O2 Lu2 O1 147.6(15) . 3_564
O2 Lu2 O1 75.57(44) . 4_666
O2 Lu2 O2 83.06(41) . 2_655
O2 Lu2 O4 110.91(51) . 1_565
O2 Lu2 O4 130.40(90) . 2_665
O2 Lu2 O6 65.94(55) . .
O2 Lu2 O6 72.92(45) . 2_655
O2 W1 O1 95.53(44) . .
O2 W1 O1 58.73(59) . 4_656
O2 W1 O2 63.86(56) . 4_666
O2 W1 O3 108.36(57) . .
O2 W1 O4 94.82(49) . .
O2 W1 O6 82.38(49) . .
O3 Lu1 O3 125.4(11) . 2_555
O3 Lu1 O4 89.90(37) . 1_565
O3 Lu1 O4 120.82(79) . 2_565
O3 Lu1 O5 71.57(60) . 1_565
O3 Lu1 O6 67.42(63) . .
O3 Lu1 O6 76.43(49) . 2_555
O3 Gd1 O3 125.4(11) . 2_555
O3 Gd1 O4 89.90(37) . 1_565
O3 Gd1 O4 120.82(79) . 2_565
O3 Gd1 O5 71.57(60) . 1_565
O3 Gd1 O6 67.42(63) . .
O3 Gd1 O6 76.43(49) . 2_555
O3 W1 O1 88.61(57) . .
O3 W1 O1 145.5(15) . 4_656
O3 W1 O2 108.36(57) . .
O3 W1 O2 58.12(82) . 4_666
O3 W1 O4 147.1(18) . .
O3 W1 O5 86.07(49) . .
O3 W1 O6 81.51(59) . .
O4 Lu3 O1 77.28(46) . 3_554
O4 Lu3 O2 91.76(40) . 2_655
O4 Lu3 O3 108.99(54) . 2_555
O4 Lu3 O5 76.01(48) . 2_555
O4 Lu3 O5 120.09(70) . 3_554
O4 Lu3 O6 69.68(53) . .
O4 Gd3 O1 77.28(46) . 3_554
O4 Gd3 O2 91.76(40) . 2_655
O4 Gd3 O3 108.99(54) . 2_555
O4 Gd3 O5 76.01(48) . 2_555
O4 Gd3 O5 120.09(70) . 3_554
O4 Gd3 O6 69.68(53) . .
O4 W1 O1 112.55(61) . .
O4 W1 O1 66.82(55) . 4_656
O4 W1 O2 94.82(49) . .
O4 W1 O3 147.1(18) . .
O4 W1 O5 75.87(55) . .
O4 W1 O6 78.77(48) . .
O5 W1 O1 75.80(50) . .
O5 W1 O1 104.50(41) . 4_656
O5 W1 O2 120.62(67) . 4_666
O5 W1 O3 86.07(49) . .
O5 W1 O4 75.87(55) . .
O5 W1 O6 108.86(57) . .
O6 Lu1 O3 67.42(63) . .
O6 Lu1 O3 76.43(49) . 2_555
O6 Lu1 O4 77.39(47) . 1_565
O6 Lu1 O5 120.75(73) . 1_565
O6 Lu1 O5 114.75(62) . 2_565
O6 Lu1 O6 95.06(44) . 2_555
O6 Gd1 O3 67.42(63) . .
O6 Gd1 O3 76.43(49) . 2_555
O6 Gd1 O4 77.39(47) . 1_565
O6 Gd1 O5 120.75(73) . 1_565
O6 Gd1 O5 114.75(62) . 2_565
O6 Gd1 O6 95.06(44) . 2_555
O6 Lu2 O1 84.44(34) . 3_564
O6 Lu2 O1 117.98(61) . 4_666
O6 Lu2 O2 65.94(55) . .
O6 Lu2 O2 72.92(45) . 2_655
O6 Lu2 O4 70.91(52) . 1_565
O6 Lu2 O6 124.15(80) . 2_655
O6 Lu3 O1 138.8(11) . 3_554
O6 Lu3 O2 76.72(46) . 2_655
O6 Lu3 O3 62.18(67) . 2_555
O6 Lu3 O3 91.21(49) . 3_564
O6 Lu3 O4 69.68(53) . .
O6 Lu3 O5 88.87(43) . 2_555
O6 Gd3 O1 138.8(11) . 3_554
O6 Gd3 O2 76.72(46) . 2_655
O6 Gd3 O3 62.18(67) . 2_555
O6 Gd3 O3 91.21(49) . 3_564
O6 Gd3 O4 69.68(53) . .
O6 Gd3 O5 88.87(43) . 2_555
O6 W1 O1 123.49(70) . 4_656
O6 W1 O2 82.38(49) . .
O6 W1 O2 110.12(49) . 4_666
O6 W1 O3 81.51(59) . .
O6 W1 O4 78.77(48) . .
O6 W1 O5 108.86(57) . .
